A High-Performance Magnesium Triflate-Based Electrolyte for Rechargeable Magnesium Batteries
Dan-Thien Nguyen,1 Alex Yong Sheng Eng,1 Man-Fai Ng,2 Vipin Kumar,1 Zdenek Sofer,3 Albertus D. Handoko,1 Gomathy Sandhya Subramanian,1 and Zhi Wei Seh1,4*
1Institute of Materials Research and Engineering, Agency for Science, Technology and Research (A*STAR), 2 Fusionopolis Way, Innovis, Singapore 138634, Singapore
2Institute of High Performance Computing, Agency for Science, Technology and Research (A*STAR), 1 Fusionopolis Way, Connexis, Singapore 138632, Singapore
3Department of Inorganic Chemistry, University of Chemistry and Technology Prague, Technická 5, 166 28 Prague 6, Czech Republic
*Correspondence: email@example.com (Z.W. Seh)
magnesium electrode. A prototype Mg battery with Mo6S8 cathode demonstrates stable cycling performance over 100 cycles. This study shows that rational design of Mg(OTf)2-based electrolytes is a promising direction towards the realization of high-performance magnesium batteries.
Rechargeable magnesium battery; nonaqueous electrolyte; magnesium
trifluoromethanesulfonate; magnesium triflate; interfacial reaction; solid electrolyte interphase; monoglyme; conditioning-free; galvanostatic Mg plating/stripping; Mo6S8
and sodium.6 These unique properties make Mg batteries attractive candidates for safer energy storage devices.
Finding an appropriate electrolyte formulation that is uniquely suitable for rechargeable magnesium batteries is one of the major technological challenges. Unlike Li-ion chemistry, in which the solid electrolyte interphase (SEI) is highly conductive to Li+ ions, spontaneous reduction of the electrolyte components on the Mg metal surface results in the formation of a passivating surface layer, which is less conductive towards Mg2+ ions. Therefore, the search for electrolyte components, particularly Mg salts, which have high reductive stability against Mg metal is crucial for improving the performance of current Mg batteries. To date, a few Mg salts allow Mg plating and stripping to occur at various degrees of reversibility. The most notable electrolyte solutions for Mg batteries are based on the organohaloaluminate complexes,7 magnesium aluminum chloride complex (MACC),8 magnesium monocarborane (Mg(CB11H12)2),9 amidomagnesium halides,10-11 and magnesium borate.12-15 However, achieving high areal capacity and high current density for Mg plating/stripping over long cycling process, which is essential for the practical use of Mg metal anode, is still challenging.16 In addition, new electrolyte systems with a simple synthetic route, based on commercially available salts and solvents, are in high demand.
anion. The ionization potential of the OTf- anion is 4.81 V, which is close to that of TFSI- (4.66 V) and ClO4- (5.04 V) anions. This suggests that Mg(OTf)2salt is also a promising salt for high voltage electrolyte system. An initial study on Mg(OTf)2-based electrolyte conducted by Lossius et al. successfully observed the deposition of Mg from an electrolyte solution of Mg(OTf)2 in dimethylacetamide.17 NuLi et al. reported reversible deposition and dissolution of magnesium from an ionic liquid-based electrolyte consisting of Mg(OTf)2 and 1-n-butyl-3-methylimidazolium tetrafluoroborate.18 However, magnesium metal passivation was reported to take place due to the negative potential limit of the ionic liquid cation.19-20 In addition, it is well established that only ethereal solvents are compatible with Mg metal anode due to their high reductive stability. However, Mg(OTf)2 has a low solubility in ethereal solvents such as glymes, resulting in their incompatibility.21 This is considered to be the biggest challenge for the development of Mg(OTf)2-based electrolyte for Mg batteries.
In this work, we carefully designed and conducted a systematic study on the combination of Mg(OTf)2 and MgCl2 salt in monoglyme (DME). Intriguingly, we found that by tuning the [Mg2+]:[Cl-] molar ratio above 1, a high concentration of Mg(OTf)2-MgCl2 can be completely dissolved into the electrolyte. The resulting electrolyte solution exhibited a superior electrochemical performance in Mg plating and stripping, showing dendrite-free deposition, high Coulombic efficiency and long cycle life (99.4% over 1000 cycles at 0.5 mA cm-2). Toward the practical use of Mg metal anode, the experiments were conducted on a conventional cell configuration using thin Celgard separator and low electrolyte volume, and tested at high current densities and high areal capacities. In addition, the deposition morphology of Mg under various current densities, the surface chemistry of the SEI formed on Mg electrode, and the electrolyte’s compatibility with Mo6S8 cathode were also carefully investigated.
RESULTS AND DISCUSSION
Homogeneous and reversible Mg deposition and dissolution
One of the greatest challenges for the utilization of Mg(OTf)2 as a salt in Mg battery electrolytes is its low solubility in ethereal solvents, especially monoglyme and diglyme, which are commonly used as solvents for Mg electrolytes due to their high reductive stability against Mg metal anode. Despite its low solubility, the galvanostatic plating/stripping of a saturated Mg(OTf)2 in DME electrolyte showed reversible plating/stripping at 0.05 mA cm-2 and 0.05 mAh cm-2 with an average Coulombic efficiency (CE) of 74.3% over 50 cycles and low overpotential of Mg plating (-0.4 V) (Figure S2). On the contrary, Mg(TFSI)2 alone in DME demonstrated poor Mg plating (Figure S3). This result suggests that Mg(OTf)2 is highly compatible with Mg metal anode and improving its solubility in DME may lead to a high-performance electrolyte solution.
demonstrates effectiveness in improving the compatibility of the electrolyte with the Mg metal anode.25-27 It should be noted here that the solubility of MgCl2 alone in DME is very low due to low chemical polarity of DME.28 Various combinations of Mg(OTf)2 and MgCl2 in DME were prepared (Figure S4) with [Mg(OTf)2]:[MgCl2] ratios ranging from 0.25 to 4, while the total concentration of Mg2+ in solution was fixed at 0.5 M. The results showed that clear and stable electrolyte solutions (i.e. complete dissolution) could be obtained at [Mg(OTf)2]:[MgCl2] ratios greater than 1, corresponding to [Mg2+]:[Cl-] ratios greater than 1 as well (Figure S4A-C). When the ratio of [Mg(OTf)2]:[MgCl2] = [Mg2+]:[Cl-] = 1, the initially-clear solution (Figure S4D) was instead unstable and crystals were formed after a few days at room temperature (Figure S4G). In mixtures where both molar ratios are less than 1, the salts were found to be insoluble (Figure S4E-F). Interestingly, a clear electrolyte can be obtained with the total concentration of Mg2+ up to 2.5 M, corresponding to the electrolyte formula of 1.5 M Mg(OTf)2 + 1 M MgCl2 in DME. Previously, Yang et al. attempted to combine Mg(OTf)2 and MgCl2 in DME at a molar ratio of 0.5 but a clear electrolyte solution was not obtainable.21 This result is consistent with our solubility findings above, which suggests that the molar ratio between Mg(OTf)2 and MgCl2 plays an unexpectedly important role in improving the solubility of their combination. At 0.5 M of Mg2+, all soluble electrolyte combinations exhibited an ionic conductivity of approximately 0.3 mS cm-1 (Table S2). The low ionic conductivity of the electrolyte solution is due to strong interaction between OTf- anion and Mg2+, similar to that observed in LiOTf-based electrolyte.29 By increasing Mg2+ concentration to 1 M, a higher ionic conductivity was obtained at 0.53 mS cm-1. However, upon further increasing the Mg2+ concentration above 1 M, we noticed the increased viscosity of the electrolyte solution, which may reduce the mobility of ions in the electrolyte solution.
were assembled using 2032-type coin cells to measure the Mg plating/stripping Coulombic efficiency of various Mg(OTf)2-MgCl2 combinations (Figure 1) to determine the optimal composition. In each cycle, a fixed areal capacity (0.1 mAh cm-2) of Mg was deposited onto the Al electrode at a current density of 0.5 mA cm-2, which was then stripped by charging the cell to 1.2 V vs. Mg/Mg2+ at the same current density. The Coulombic efficiency for each cycle was calculated based on the ratio of the capacity of stripped Mg to that of plated Mg. Amongst the three stable electrolyte combinations, 0.3 M Mg(OTf)2 + 0.2 M MgCl2 in DME demonstrated the highest average Coulombic efficiency of 99.4% for 1000 cycles. The cell also shows an initial Coulombic efficiency (ICE) of 89.9% and reached 95.8% in the second cycle. In addition, it also exhibited the lowest Mg plating and stripping overpotential at -0.17 V and +0.17 V (Figure S5), respectively. It should be noted that all electrolyte combinations with Mg2+concentration of 0.5 M have similar ionic conductivity, implying that the improved cycling performance of 0.3 M Mg(OTf)2 + 0.2 M MgCl2 in DME is related to the concentration of chloride in the electrolyte. It is well-established that MgCl2 plays a crucial role in enhancing Mg plating/stripping: it can inhibit Mg surface passivation through the formation of adsorbed Cl- and/or MgCl2 on the Mg surface as well as through a dynamic competition with adventitious H2O impurity in the double layer.30
among the solutions tested. For comparison, a similar experiment was performed on 0.25 M Mg(TFSI)2 + 0.5 MgCl2 in DME electrolyte, which is a common formula used in Mg(TFSI)2-based system (Figure S6).27 The asymmetric cell showed an average CE of 94.0 % and a cycle life of around 100 cycles, lower than our developed electrolytes, which indicates the superior performance of Mg(OTf)2 salt to Mg(TFSI)2.
In order to obtain a thorough understanding of Mg(OTf)2-MgCl2 electrolyte performance, we conducted various electrochemical characterizations as shown in Figures 1B-E. A typical cyclic voltammogram measured with Pt working electrode in 0.3 M Mg(OTf)2 + 0.2 M MgCl2 in DME (Figure 1B) exhibited highly reversible and conditioning-free Mg plating/stripping. The first cycle demonstrated a large Mg deposition overpotential at -1.0 V vs. Mg/Mg2+, but it quickly reduced to -0.3 V in the second cycle, which is well consistent with voltage profiles of the galvanostatic cycling in Figure 1D. The large overpotential in the first cycle was probably due to the elimination of thin MgO oxide on Mg anode, which was formed by the reduction of trace moisture from the glovebox and/or the reduction of impurities during the first cathodic scan. The first positive scan exhibited a large cathodic peak, beginning near 0 V vs. Mg/Mg2+. In subsequent cycles, the cyclic voltammogram showed highly reversible Mg deposition and dissolution with low Mg deposition overpotential (-0.3 V) and high cathodic peak in the positive scan. The anodic stability of 0.3 M Mg(OTf)2 + 0.2 M MgCl2 in DME was further studied by linear sweep voltammetry using inert Pt electrode and non-noble metal electrodes (Figure 1C). On the inert Pt electrode, the onset of the electrolyte oxidation appeared at 3.0 V vs. Mg/Mg2+, which is close to that of Mg(TFSI)2-MgCl2 system reported by Aurbach’s group.27 On non-noble metal electrodes, including Al, stainless steel (SS), Ni, and Mo, the oxidation current began to increase at 1.9 V, 2.0 V, 2.4 V, and 3.1 V, respectively due to chloride corrosion.
the asymmetric cell shows an overpotential of -0.4 V vs. Mg/Mg2+ (Figure 1D), which is probably due to the elimination of the thin MgO layer on Mg metal anode. The first Mg dissolution showed a low overpotential at 0.2 V vs. Mg/Mg2+ and delivers a CE of 84.8%. The irreversible capacity corresponds to the reduction of trace moisture and impurities presented in electrolyte and cell components. In subsequent cycles, the Mg deposition and dissolution overpotentials were reduced and well-maintained near ±0.2 V over 100 cycles. The CE was 97.3% in the second cycle, reached 99.1% by the 7th cycle, and stabilized at 99% over 100 cycles, indicating a typical behavior of a conditioning-free electrolyte system. The cell delivered an average CE of 99.1% over 100 cycles. At 1 mA cm-2 and 1 mAh cm-2, the asymmetric cell also demonstrated an excellent Mg plating/stripping with average CE of 99.2% (Figure S7). This electrolyte system demonstrated a significant performance enhancement compared to other Mg(OTf)2 electrolyte systems reported in literature and is highly competitive with other reported systems (Table S3), especially in terms of Coulombic efficiency, areal capacity and current density.21-22 It should be noted here that the excellent cycling performance of the asymmetric cell using 0.3 M Mg(OTf)2 + 0.2 M MgCl2 in DME electrolyte was achieved using an experimental setup that is close to the practical requirement of batteries such as the use of thin Celgard separators, unlike the majority of other works which use glass fiber separators.13, 15-16, 22, 32 In addition, we also demonstrate low electrolyte volume (25 μl per coin cell), relatively high current density (0.5 to 1 mA cm-2), and areal capacity of 0.5 to 1 mAh cm -2 as indicated in Table S3.
was also performed on the Mg deposits (Figure 2C) to confirm its crystal structure. The measurement was conducted on Mg film plated at 0.5 mA cm-2 and 3 mAh cm-2. The XRD pattern clearly confirmed that the agglomerated deposits are pure Mg polycrystalline in nature (PDF Card No. 00-001-1141). EDX spectrum (Figure 2D) and elemental mapping (Figure S8) of the sample confirms that the Mg deposits were of high purity with Mg content of 91.6%. Other elements such as C, O, F, S, Cl, and Al were also present but at very low percentages (Figure S8).
and 99.4%, respectively. This result suggests that Mg deposition and dissolution occurred at very high reversibility with similar overpotentials even at high areal capacity up to 5 mAh cm -2.
decrease of the cell impedance with cycle number, which is due to the elimination of surface oxide and formation of fresh Mg metal by repeated deposition/dissolution. A similar observation was also reported by Zhao-Karger et al. in the magnesium tetrakis(hexafluoroisopropyloxy) borate electrolyte.15
Due to the inherent nature of the electrochemical deposition process, dendritic structures typically form when a high current density is applied to deposit metals. In the case of Mg, the maximum current density limit that allows for dendrite-free Mg plating is highly dependent on the electrolyte solution used. Thus, it is important to determine this current density limit to avoid the dendritic growth of Mg with our electrolyte system.35 Figure 4H presents the voltage vs. time curve of an Mg//Mg symmetric cell cycled at 0.5 mAh cm-2 with current density gradually increased from 0.5 mA cm-2 to 3 mA cm-2. The overpotential increased from 0.17 V at 0.5 mA cm-2 to 0.3 V at 1 mA cm-2, and 0.5 V at 2 mA cm-2. Even at high current densities, the symmetric cell showed flat potential curves during plating/stripping, implying a smooth Mg cycling process. At a current density of 3 mA cm-2, the overpotential increased significantly to 0.8 V and a short circuit occurred in the 3rd cycle. The SEM images show a significant change in the shape of Mg deposits to a dendritic structure at 3 mA cm-2 (Figure S10). This result suggests that the limiting current density for dendrite-free deposition in our electrolyte is 2 mA cm-2. It is worth noting that this limiting current could be improved by enhancing the ionic conductivity of the electrolyte solution, which will be reported in future work.
the stripped state (Figure 5C and D), the Mg deposits from previous cycles were completely removed and a clean surface was observed. In both cases, the electrode surface became uneven but shows no dendritic structure formation as illustrated in Figure 5E. To further analyze the Mg deposition morphology, we acquired a cross-section SEM image of an Mg electrode after Mg deposition (Figure 5F). The film appears to be dense and uniform with an average thickness of 13.3 μm at 3 mAh cm-2.
Formation of a robust solid electrolyte interphase on Mg anode
Since the Mg anode-electrolyte interface is crucial to the reversibility of the Mg plating/stripping process, we carried out X-ray photoelectron spectroscopy (XPS) in depth profiling mode to examine the surface physiochemistry of Mg metal anode from the top surface to the bulk of the SEI. Figure 6 presents the XPS spectra obtained from the Mg metal electrode from a symmetric cell after 20 cycles at the current density of 0.5 mA cm-2 and areal capacity of 0.5 mAh cm-2. The electrode was removed from a coin cell in the plated state to be examined under XPS analysis, carefully avoiding any ambient contamination or decomposition of surface species as described in the experimental section. Due to the weak C 1s signal, all spectra herein were calibrated using the Mg 2p peak of Mg0 at 49.8 eV.36
surface film contained both organic species (ether and ester moieties), inorganic components (MgO, Mg(OH)2, MgF2, MgS, MgCl2), and adsorbed chloride-containing components.
here that the surface film on Mg metal anode consists of organic and adsorbed chloride-containing species on the top surface, and mostly inorganic components such as MgO, Mg(OH)2, MgCO3, MgS, MgCl2, and MgF2 within the interior (Figure S11B). This largely inorganic surface film plays an important role in enabling the reversibility of Mg deposition and dissolution. It is well known that solid phases such as MgF2 or MgO are not conductive to Mg2+ due to its high charge density. Since high reversibility is still observed at the Mg anode, we propose that the inorganic layer is not entirely compact; instead it contains pinholes that allow Mg2+ diffusion, similar to that of hexafluorophosphate-based solutions reported by Aurbach’s group.55 The chloride is expected to play an important role in engineering the structure and composition of this layer. Further investigation on the structure and Mg mobility through this SEI will be reported in future work.
Electrochemical performance of Mg//Mo6S8 full-cell
capacity of 75 mAh g-1 and stable cycling performance over 100 cycles with a capacity retention of 90.8% at 0.1 C, indicating high compatibility with cathode materials up to 2.2 V. The electrolyte appears to be promising for future development of Mg battery by combining with high capacity and fast kinetic cathode materials such as metal chalcogenide cathodes.60-61
Reaction mechanism of Mg(OTf)2 and MgCl2 in DME
In order to explain the improved solubility of Mg(OTf)2 and MgCl2 combination in DME, we conducted a structural analysis of the electrolyte solution using single-crystal XRD (SCXRD) (Figure 8) and Raman spectroscopy (Figure 9). To induce crystal precipitation, an electrolyte with a high concentration of 1.5 M Mg(OTf)2 + 1 M MgCl2 in DME solution was prepared to grow the single crystal. The single-crystal structure refinement yielded the structure shown in Figure 8 and Table S5. The single-crystal structure with the formula Mg(DME)2(OTf)2 clearly shows an Mg2+ cation encaged by two DME molecules and two OTf- anions without any coordination to chloride ions. Mg(OTf)2 acquires a V-shape with an equilibrium angle of 91.51o between the oxygen atoms of the triflate group (Figure 8). This structure is similar to that of MgCl2 in DME, which forms MgCl2(DME)2 solution species.62-63
vibrational mode at 773 cm-1 to 762 cm-1 and the blue shift of vibrational mode at 1038 cm-1 to 1049 cm-1 of triflate anion (Figure 9C). In addition, we also observed the presence of free OTf -anion, evidenced by the signals at 311 and 346 cm-1. The Raman spectrum of 1-butyl-3-methylimidazolium trifluoromethanesulfonate ([BMIM][OTf]) and DME (1:5 vol. ratio) solution (Figure 9D) supported this assignment. The absence of chloride-containing species in Raman spectra suggest that Cl- might form cation that is not detectable by Raman spectroscopy such as [MgCl]+. 35Cl nuclear magnetic resonance (NMR) measurements showed that these solutions contain no free chloride ions (Figure S14). Characterization of the electroactive complex, especially chloride-containing species, would require extensive research and will be the subject of future studies.
of the OTf- than that of TFSI- anion also allows it to coordinate into the octahedral structure of the Mg complex. Herein, we propose the following possible reaction schemes of Mg(OTf)2 and MgCl2 in DME solution (Equations 1-5):
Mg(OTf)2 + 2DME Mg(OTf)2(DME)2 (1)
Mg(OTf)2(DME)2 + DME [Mg(DME)3]2+ + 2OTf- (2)
MgCl2 + 2DME MgCl2(DME)2 (3)
[Mg(DME)3]2++ MgCl2(DME)2 [Mg2Cl2(DME)4]2+ + DME (4) [Mg2Cl2(DME)4]2+ 2[MgCl(DME)x]+ + (4-2x)DME (5)
Equations 1 and 2 illustrate the interactions between Mg(OTf)2 and DME, forming Mg(OTf)2(DME)2 and possibly [Mg(DME)3]2+ cation. In the electrolyte solution containing only Mg(OTf)2, Equation (2) might be negligible due to the strong interaction between Mg2+ and OTf- anion as explained above, corresponding to the low solubility of Mg(OTf)2 alone in DME. The presence of MgCl2 leads to the occurrence of reactions (3) to (5) as suggested by Aurbach’s group.62-63 These reactions effectively increase the dissociation of Mg(OTf)2 (Equation 2) into more soluble species such as [Mg(DME)3]2+ and [MgCl(DME)x]+. The formation of complexes such as [MgCl(OTf)(DME)2] also cannot be ruled out. The formation of these species might well explain the enhanced solubility of Mg(OTf)2 with the addition of MgCl2. However, since the [Mg2+]:[Cl-] ratio is above 1 in all the electrolyte solutions, a large portion of Mg2+ ions exist as Mg(OTf)2(DME)2 and possibly [Mg(DME)3]2+. Therefore, the crystallization of the electrolyte solution yielded only the formation of Mg(OTf)2(DME)2 probably due to its charge-neutral nature, which made it less soluble than other complexes. Further structural analysis of Mg complexes in this electrolyte system will be reported in future work.
In this work, we report for the first time that the simple combination of Mg(OTf)2 and MgCl2 in DME with a [Mg2+]:[Cl-] ratio larger than 1 exhibits highly reversible and conditioning-free Mg dissolution/deposition (99.4% Coulombic efficiency over 1000 cycles) at room temperature. In addition, the electrolyte is promising for practical applications at high areal capacity (5 mAh cm-2)and high current density (3 mA cm-2) while maintaining high CE at 99.4% and 98.4%, respectively. Investigation on the surface chemistry of Mg anode reveals the formation of a surface film, which consists of organic and adsorbed chloride-containing species on the top surface, and mostly Mg-based inorganic components in the interior. This largely inorganic and robust SEI structure enables reversible Mg deposition and dissolution at high Coulombic efficiency. This work provides new insights on the rational design of promising electrolyte systems for rechargeable magnesium batteries, which can be extended to other energy storage systems beyond Li-ion batteries in the future.
EXPERIMENTAL PROCEDURES Resource Availability
Further information and requests for resources and reagents should be directed to and will be fulfilled by the Lead Contact, Prof. Zhi Wei Seh (firstname.lastname@example.org).
Materials synthesized in this manuscript can be obtained by request to the Lead Contact.
Data and Code Availability
All data are available from the corresponding author upon reasonable request.
MgCl2 (99.99%), molecular sieve (3Å beads, 4-8 mesh), 1,2-dimethoxyethane (DME, 99.5%), N-Methyl-2-pyrrolidone (NMP, 99.5%), and poly(vinylidene fluoride) (PVdF, Mw ~ 534,000) were purchased from Sigma-Aldrich. Mg(OTf)2 (99.5%) and Mg(TFSI)2 (99.5%) were purchased from Solvionic. Carbon black (99%) and platinum foil (99.99%) were purchased from Alfa Aesar. Mg foil (>99%, 0.1 mm thick) was purchased from MTI.
Molecular sieves were dried at 200 oC for 24 h in the oven followed by vacuum drying overnight, and finally stored in an Ar-filled glovebox. DME was dried with molecular sieves for at least 24 h prior to electrolyte preparation. A predetermined amount of Mg(OTf)2 and MgCl2 powders were weighted directly into a glass vial, followed by addition of DME solvent and stir bar. The mixture was stirred for 24 h at 60 oC. The solution was rested overnight and a trace amount of white solid powder at the bottom of glass vial was removed. Finally, molecular sieves were added into the electrolyte solution to further remove moisture from the electrolyte solution. The moisture content in all electrolyte solutions is determined to be less than 20 ppm using Karl Fischer Coulometer C30X (Mettler Toledo). The ionic conductivity of the electrolyte solution was measured using Fisherbrand Accumet AB200 at room temperature.
Cell configurations and electrochemical characterization
between OCV and 6.0 V vs. Mg/Mg2+. All cell assembly and voltammetry measurements were conducted in an Ar-filled glove box (H2O < 0.1 ppm, and O2 < 1 ppm).
Galvanostatic plating/stripping was performed using a 2032-type coin cell. In the asymmetric cell configuration, the coin cell consists of a carbon-coated Al disk (Figure S16) (1 cm2) as the working electrode, polished Mg disk (1.26 cm2) as the counter electrode, and 2 layers of Celgard separators. The cell was filled with 25 μl of the electrolyte solution. It should be noted here that in our experiments with various working electrodes, including carbon-coated Al, Cu, stainless steel, nickel, and titanium, the highest plating/stripping Coulombic efficiency was achieved with carbon-coated Al foil. In the symmetric cell configuration, the Al disk was replaced with polished Mg disks (1.26 cm2). All coin cell components were washed with isopropanol and acetone, and dried overnight in 60 oC oven. Celgard separators (16 mm in diameter) were punched out and dried in vacuum at 60oC for three days, and stored in an Ar-filled glovebox prior to cell assembly. Galvanostatic plating of Mg was carried out at the desired current density and areal capacity, followed by stripping of Mg by charging to a cutoff voltage of 1.2 V vs. Mg/Mg2+, all performed at room temperature. The Coulombic efficiency for each cycle was calculated as the ratio of the capacity of Mg stripped to that of Mg deposited. Electrochemical impedance spectroscopy was carried out on symmetric Mg//Mg cell before cycling, after the first plating/stripping cycle, after 20 and 50 cycles using Gamry potentiostat between 1 MHz to 10 mHz. The full cell Mg//Mo6S8 was cycled between 0.2 - 2.2 V using constant current-constant voltage mode (CC-CV mode) at a current density of 0.1 C after a formation process, which includes one discharge-charge cycle at 0.05 C followed by discharge to 0.2 V at 0.1 C. The C rate was calculated based on the theoretical capacity of Mo6S8 at 129 mAh g-1 (1 C = 129 mA g-1). The Coulombic efficiency of Mg//MgMo6S8 cell for each cycle was calculated based on the ratio of discharge capacity to charge capacity.
Single crystals were obtained by layering hexane on the top of 1.5 M Mg(OTf)2 + 1 M MgCl2 in DME solution (0.5 ml) in 1 ml glass vial. The sample then was placed in an Ar-filled glovebox for 7 days. Intensity data were collected at 100 K using Mo-Kα radiation (λ = 0.71073 Å) on a Bruker D8 Quest diffractometer with an Incoatec microfocus X-ray Source. The collected frames were processed with the software SAINT.65 The data were corrected for absorption by using the SADABS program.66 The structure was solved by the Direct methods and refined by full-matrix least-squares analyses on F2 (SHELXL-2018/3).67 All non-hydrogen atoms were refined anisotropically. The positions of all hydrogen atoms were generated geometrically and allowed to ride on their respective parent carbon atoms before the final cycle of least-squares refinement. A Renishaw inVia confocal microscope was employed for Raman spectroscopy, using a 532 nm excitation laser in backscattering geometry. Samples (1 ml of electrolyte solution or powder) were sealed in a glass tube filled with Ar.
After cycling, coin cells were disassembled in Ar-filled glovebox. The electrodes were washed with dried DME to remove residual electrolyte for 30 seconds and dried overnight at room temperature. The Mg deposition morphology was studied using SEM (JEOL 7600F) at an accelerating voltage of 5 kV. The electrode was mounted on the SEM sample holder in an Ar-filled glovebox and transferred to the analysis chamber using an airtight carrier. The crystal structure information of Mg deposits was revealed by D8 Advance, Bruker, X-ray diffractometer (XRD), and the materials were scanned between 10 and 70o (2θ) using Cu Kα radiation. The Mg deposited electrode was mounted in an airtight specimen holder (Bruker).
exposing the sample to air during transfer from the Ar-filled glovebox to the XPS analysis chamber. The sample was vacuumed overnight to remove gases and absorbed solvent. XPS measurement was conducted within 18 h after removal from the coin cell to minimize the decomposition of surface species. Due to the weak signal of C 1s spectra, herein all spectra were calibrated using Mg 2p peak of Mg0 at 49.8 eV. The chemical composition of the interphase as a function of its thickness was characterized using XPS depth profiling, conducted at 3 kV (ion-beam current of 2 μA) for 30 s, 1 min, 2 min, 5 min, 8 min, and 15 min.
Synthesis of Mo6S8 and cathode preparation
Chevrel phase Cu2Mo6S8 was first synthesized as described in the literature.56 The Cu2Mo6S8 powder was then underwent a chemical leaching process to yield the final product of Mo6S8 as follows: 600 mg of Cu2Mo6S8 was added into 40 ml 8 M HCl solution. The mixture was then stirred for 8 h at room temperature with dried air bubbling. The crystal structure of Cu2Mo6S8 and Mo6S8 was confirmed by XRD. Mo6S8 cathode slurry was prepared by mixing active material, carbon black, and PVdF in the weight ratio of 80:10:10 in NMP solvent using Thinky Mixer (ARE-250) for 20 minutes. The slurry was then coated on Ni foil and dried at 60oC for 12 h and 120 oC for 6 h. The electrodes were then punched into 12 mm-diameter disks and dried at 120 oC in a vacuum oven prior to use. The total electrode loading mass is 8.8 mg cm2 (7.0 mg cm-2 for Mo6S8).
Document S1. Supplemental Experimental Procedures, Figures S1–S16, and Table S1-S5.
performance computing facilities. Z.S. was supported by Czech Science Foundation (GACR No. 20-16124J).
Dan-Thien Nguyen: Conceptualization, Data curation, Formal analysis, Investigation, Writing - original draft. Alex Yong Sheng Eng: Data curation, Formal analysis, Investigation. Man-Fai Ng: Investigation, Software. Vipin Kumar: Data curation, Formal analysis, Investigation. Zdenek Sofer: Data curation, Formal analysis, Investigation. Albertus D. Handoko: Data curation, Formal analysis, Investigation. Gomathy Sandhya Subramanian: Formal analysis, Investigation. Zhi Wei Seh: Conceptualization, Supervision, Writing - original draft.
DECLARATION OF INTERESTS
The authors declare that they have no competing interests.
1. Muldoon, J., Bucur, C. B., and Gregory, T. (2014). Quest for nonaqueous multivalent secondary batteries: Magnesium and beyond. Chem. Rev. 114, 11683-11720.
2. Canepa, P., Sai Gautam, G., Hannah, D. C., Malik, R., Liu, M., Gallagher, K. G., Persson, K. A., and Ceder, G. (2017). Odyssey of multivalent cathode materials: Open questions and future challenges. Chem. Rev. 117, 4287-4341.
3. Choi, J. W., and Aurbach, D. (2016). Promise and reality of post-lithium-ion batteries with high energy densities. Nat. Rev. Mater. 1, 16013.
4. Aurbach, D., Cohen, Y., and Moshkovich, M. (2001). The study of reversible
magnesium deposition by in situ scanning tunneling microscopy. Electrochem. Solid-State Lett. 4, A113-A116.
5. Kumar, V., Wang, Y., Eng, A. Y. S., Ng, M.-F., and Seh, Z. W. (2020). A biphasic interphase design enabling high performance in room temperature sodium-sulfur batteries. Cell Rep. Phys. Sci. 1, 100044.
6. Jäckle, M., and Groß, A. (2014). Microscopic properties of lithium, sodium, and magnesium battery anode materials related to possible dendrite growth. J. Chem. Phys. 141, 174710.
7. Aurbach, D., Lu, Z., Schechter, A., Gofer, Y., Gizbar, H., Turgeman, R., Cohen, Y., Moshkovich, M., and Levi, E. (2000). Prototype systems for rechargeable magnesium batteries. Nature. 407, 724-727.
9. Tutusaus, O., Mohtadi, R., Arthur, T. S., Mizuno, F., Nelson, E. G., and Sevryugina, Y. V. (2015). An efficient halogen-free electrolyte for use in rechargeable magnesium batteries. Angew. Chem. Int. Ed. 54, 7900-7904.
10. Liebenow, C., Yang, Z., and Lobitz, P. (2000). The electrodeposition of magnesium using solutions of organomagnesium halides, amidomagnesium halides and magnesium organoborates. Electrochem. Commun. 2, 641-645.
11. Kim, H. S., Arthur, T. S., Allred, G. D., Zajicek, J., Newman, J. G., Rodnyansky, A. E., Oliver, A. G., Boggess, W. C., and Muldoon, J. (2011). Structure and compatibility of a magnesium electrolyte with a sulphur cathode. Nat. Commun. 2, 427.
12. Zhang, Z., Cui, Z., Qiao, L., Guan, J., Xu, H., Wang, X., Hu, P., Du, H., Li, S., Zhou, X., et al. (2017). Novel design concepts of efficient Mg-ion electrolytes toward high-performance magnesium–selenium and magnesium–sulfur batteries. Adv. Energy Mater. 7, 1602055.
13. Zhao-Karger, Z., Gil Bardaji, M. E., Fuhr, O., and Fichtner, M. (2017). A new class of non-corrosive, highly efficient electrolytes for rechargeable magnesium batteries. J. Mater. Chem. A. 5, 10815-10820.
14. Du, A., Zhang, Z., Qu, H., Cui, Z., Qiao, L., Wang, L., Chai, J., Lu, T., Dong, S., Dong, T., et al. (2017). An efficient organic magnesium borate-based electrolyte with non-nucleophilic characteristics for magnesium–sulfur battery. Energy Environ. Sci. 10, 2616-2625.
15. Zhao-Karger, Z., Liu, R., Dai, W., Li, Z., Diemant, T., Vinayan, B. P., Bonatto Minella, C., Yu, X., Manthiram, A., Behm, R. J., et al. (2018). Toward highly reversible
magnesium–sulfur batteries with efficient and practical mg[b(hfip)4]2 electrolyte. ACS Energy Lett. 3, 2005-2013.
16. Tang, K., Du, A., Dong, S., Cui, Z., Liu, X., Lu, C., Zhao, J., Zhou, X., and Cui, G. (2020). A stable solid electrolyte interphase for magnesium metal anode evolved from a bulky anion lithium salt. Adv. Mater. 32, 1904987.
17. Lossius, L. P., and Emmenegger, F. (1996). Plating of magnesium from organic solvents. Electrochim. Acta. 41, 445-447.
18. NuLi, Y., Yang, J., and Wu, R. (2005). Reversible deposition and dissolution of magnesium from BMIMBF4 ionic liquid. Electrochem. Commun. 7, 1105-1110. 19. Amir, N., Vestfrid, Y., Chusid, O., Gofer, Y., and Aurbach, D. (2007). Progress in
nonaqueous magnesium electrochemistry. J. Power Sources. 174, 1234-1240.
20. Cheek, G. T., O’Grady, W. E., El Abedin, S. Z., Moustafa, E. M., and Endres, F. (2008). Studies on the electrodeposition of magnesium in ionic liquids. J. Electrochem. Soc. 155, D91-D95.
21. Yang, Y., Wang, W., Nuli, Y., Yang, J., and Wang, J. (2019). High active magnesium trifluoromethanesulfonate-based electrolytes for magnesium-sulfur batteries. ACS Appl. Mater. Interfaces. 11, 9062-9072.
22. Huang, D., Tan, S., Li, M., Wang, D., Han, C., An, Q., and Mai, L. (2020). Highly efficient non-nucleophilic Mg(CF3SO3)2-based electrolyte for high-power Mg/S battery. ACS Appl. Mater. Interfaces. 12, 17474-17480.
23. Bieker, G., Salama, M., Kolek, M., Gofer, Y., Bieker, P., Aurbach, D., and Winter, M. (2019). The power of stoichiometry: Conditioning and speciation of MgCl2/AlCl3 in tegdme-based electrolytes. ACS Appl. Mater. Interfaces. 11, 24057-24066.
25. Liu, T., Shao, Y., Li, G., Gu, M., Hu, J., Xu, S., Nie, Z., Chen, X., Wang, C., and Liu, J. (2014). A facile approach using MgCl2 to formulate high performance Mg2+ electrolytes for rechargeable Mg batteries. J. Mater. Chem. A. 2, 3430.
26. Liao, C., Sa, N., Key, B., Burrell, A. K., Cheng, L., Curtiss, L. A., Vaughey, J. T., Woo, J.-J., Hu, L., Pan, B., et al. (2015). The unexpected discovery of the Mg(HMDS)2/MgCl2 complex as a magnesium electrolyte for rechargeable magnesium batteries. J. Mater. Chem. A. 3, 6082-6087.
27. Shterenberg, I., Salama, M., Yoo, H. D., Gofer, Y., Park, J.-B., Sun, Y.-K., and
Aurbach, D. (2015). Evaluation of (CF3SO2)2N−(TFSI) based electrolyte solutions for Mg batteries. J. Electrochem. Soc. 162, A7118-A7128.
28. Watahiki, T., Kiyosu, T., and Okamoto, K. (2016). Electrolyte solution for electrochemical devices. US patent No. 9,263,767.
29. Webber, A. (1991). Conductivity and viscosity of solutions of LiCF3SO3, Li(CF3SO2)2N, and their mixtures. J. Electrochem. Soc. 138, 2586-2590.
30. Connell, J. G., Genorio, B., Lopes, P. P., Strmcnik, D., Stamenkovic, V. R., and Markovic, N. M. (2016). Tuning the reversibility of Mg anodes via controlled surface passivation by H2O/Cl– in organic electrolytes. Chem. Mater. 28, 8268-8277.
31. Lapidus, S. H., Rajput, N. N., Qu, X., Chapman, K. W., Persson, K. A., and Chupas, P. J. (2014). Solvation structure and energetics of electrolytes for multivalent energy storage. Phys. Chem. Chem. Phys. 16, 21941-21945.
32. Kang, J., Lim, C., Kim, H., Heo, J. W., Hwang, S., Jang, M., Yang, D., Hong, S.-T., and Lee, H. (2017). Non-grignard and lewis acid-free sulfone electrolytes for rechargeable magnesium batteries. Chem. Mater. 29, 3174-3180.
33. Yoo, H. D., Liang, Y., Li, Y., and Yao, Y. (2015). High areal capacity hybrid
magnesium–lithium-ion battery with 99.9% Coulombic efficiency for large-scale energy storage. ACS Appl. Mater. Interfaces. 7, 7001-7007.
34. He, Y., Li, Q., Yang, L., Yang, C., and Xu, D. (2019). Electrochemical-conditioning-free and water-resistant hybrid AlCl3/MgCl2 /Mg(TFSI)2 electrolytes for rechargeable magnesium batteries. Angew. Chem. Int. Ed. Engl. 58, 1-6.
35. Bonnick, P., and Muldoon, J. (2020). A trip to oz and a peak behind the curtain of magnesium batteries. Adv. Funct. Mater. n/a, 1910510.
36. Wanger, C., Riggs, W., Davis, L., Moulder, J., and Muilenberg, G. (1979). Handbook of X-ray Photoelectron Spectroscopy: A reference book of standard data for use in X-ray photoelectron spectroscopy. Eden Prairie, MN: Physical Electronics Division, Perkin-Elmer Corp.
37. Nguyen, D.-T., and Song, S.-W. (2017). Magnesium stannide as a high-capacity anode for magnesium-ion batteries. J. Power Sources. 368, 11-17.
38. Yu, Y., Baskin, A., Valero-Vidal, C., Hahn, N. T., Liu, Q., Zavadil, K. R., Eichhorn, B. W., Prendergast, D., and Crumlin, E. J. (2017). Instability at the electrode/electrolyte interface induced by hard cation chelation and nucleophilic attack. Chem. Mater. 29, 8504-8512.
39. Nguyen, C. C., and Lucht, B. L. (2014). Comparative study of fluoroethylene carbonate and vinylene carbonate for silicon anodes in lithium ion batteries. J. Electrochem. Soc. 161, A1933-A1938.
40. Wong, P. C., Li, Y. S., and Mitchell, K. A. R. (1995). Investigations of the interface between magnesium and polyethyleneterephthalate by X-ray photoelectron
spectroscopy. Appl. Surf. Sci. 84, 245-252.
42. Tie, D., Feyerabend, F., Hort, N., Willumeit, R., and Hoeche, D. (2010). XPS studies of magnesium surfaces after exposure to Dulbecco's modified eagle medium, Hank's buffered salt solution, and simulated body fluid. Adv. Eng. Mater. 12, B699-B704. 43. Kamarulzaman, N., Chayed, N. F., Badar, N., Kasim, M. F., Mustaffa, D. T., Elong, K.,
Rusdi, R., Oikawa, T., and Furukawa, H. (2016). Band gap narrowing of 2-D ultra-thin MgO graphene-like sheets. ECS J. Solid State Sci. Technol. 5, Q3038-Q3045.
44. Zhao, X., Li, Q., Zhao-Karger, Z., Gao, P., Fink, K., Shen, X., and Fichtner, M. (2014). Magnesium anode for chloride ion batteries. ACS Appl. Mater. Interfaces. 6, 10997-11000.
45. Gofer, Y., Turgeman, R., Cohen, H., and Aurbach, D. (2003). XPS investigation of surface chemistry of magnesium electrodes in contact with organic solutions of organochloroaluminate complex salts. Langmuir. 19, 2344-2348.
46. Seh, Z. W., Sun, J., Sun, Y., and Cui, Y. (2015). A highly reversible room-temperature sodium metal anode. ACS Cent Sci. 1, 449-55.
47. Agostini, M., Xiong, S., Matic, A., and Hassoun, J. (2015). Polysulfide-containing glyme-based electrolytes for lithium sulfur battery. Chem. Mater. 27, 4604-4611. 48. Briggs, D., and Beamson, G. (1993). Xps studies of the oxygen 1s and 2s levels in a
wide range of functional polymers. Anal. Chem. 65, 1517-1523.
49. López, G. P., Castner, D. G., and Ratner, B. D. (1991). XPS O 1s binding energies for polymers containing hydroxyl, ether, ketone and ester groups. Surf. Interface Anal. 17, 267-272.
50. Merrill, L. C., and Schaefer, J. L. (2019). The influence of interfacial chemistry on magnesium electrodeposition in non-nucleophilic electrolytes using sulfone-ether mixtures. Front. Chem. 7, 194.
51. Magni, E., and Somorjai, G. A. (1996). Preparation of a model ziegler-natta catalyst: Electron irradiation induced titanium chloride deposition on magnesium chloride thin films grown on gold. Surf. Sci. 345, 1-16.
52. Ding, M. S., Diemant, T., Behm, R. J., Passerini, S., and Giffin, G. A. (2018). Dendrite growth in Mg metal cells containing Mg(TFSI)2/glyme electrolytes. J. Electrochem. Soc. 165, A1983-A1990.
53. Kumar, V., Eng, A. Y. S., Wang, Y., Nguyen, D.-T., Ng, M.-F., and Seh, Z. W. (2020). An artificial metal-alloy interphase for high-rate and long-life sodium–sulfur batteries. Energy Storage Mater. 29, 1-8.
54. Jie, Y., Liu, X., Lei, Z., Wang, S., Chen, Y., Huang, F., Cao, R., Zhang, G., and Jiao, S. (2020). Enabling high-voltage lithium metal batteries by manipulating solvation
structure in ester electrolyte. Angew. Chem. Int. Ed. 59, 3505-3510.
55. Shterenberg, I., Salama, M., Gofer, Y., and Aurbach, D. (2017). Hexafluorophosphate-based solutions for mg batteries and the importance of chlorides. Langmuir. 33, 9472-9478.
56. Lancry, E., Levi, E., Gofer, Y., Levi, M., Salitra, G., and Aurbach, D. (2004). Leaching chemistry and the performance of the Mo6S8 cathodes in rechargeable Mg batteries. Chem. Mater. 16, 2832-2838.
57. Cheng, Y., Stolley, R. M., Han, K. S., Shao, Y., Arey, B. W., Washton, N. M., Mueller, K. T., Helm, M. L., Sprenkle, V. L., Liu, J., et al. (2015). Highly active electrolytes for rechargeable mg batteries based on a [Mg2(μ-Cl)2]2+ cation complex in
dimethoxyethane. Phys. Chem. Chem. Phys. 17, 13307-13314.
59. Saha, P., Jampani, P. H., Datta, M. K., Okoli, C. U., Manivannan, A., and Kumta, P. N. (2014). A convenient approach to Mo6S8 Chevrel phase cathode for rechargeable magnesium battery. J. Electrochem. Soc. 161, A593-A598.
60. Xue, X., Chen, R., Yan, C., Zhao, P., Hu, Y., Kong, W., Lin, H., Wang, L., and Jin, Z. (2019). One-step synthesis of 2-ethylhexylamine pillared vanadium disulfide
nanoflowers with ultralarge interlayer spacing for high-performance magnesium storage. Adv. Energy Mater. 9, 1900145.
61. Pei, C., Yin, Y., Sun, R., Xiong, F., Liao, X., Tang, H., Tan, S., Zhao, Y., An, Q., and Mai, L. (2019). Interchain-expanded vanadium tetrasulfide with fast kinetics for rechargeable magnesium batteries. ACS Appl. Mater. Interfaces. 11, 31954-31961. 62. Neumüller, B., Stieglitz, G., and Dehnicke, K. (1993). Crystal structure of MgCl2(1,
2-dimethoxyethane)2. Z. Naturforsch. B. 48, 1151-1154.
63. Salama, M., Shterenberg, I., J.W. Shimon, L., Keinan-Adamsky, K., Afri, M., Gofer, Y., and Aurbach, D. (2017). Structural analysis of magnesium chloride complexes in
dimethoxyethane solutions in the context of Mg batteries research. J. Phys. Chem. C. 121, 24909-24918.
64. Saito, M., Yamada, S., Ishikawa, T., Otsuka, H., Ito, K., and Kubo, Y. (2017). Factors influencing fast ion transport in glyme-based electrolytes for rechargeable lithium–air batteries. RSC Adv. 7, 49031-49040.
65. Smart, Saint+ for Windows NT (version 6.02a) (1998). Area detector control and integration software, Bruker AXS Inc., Madison, WI (USA).
66. Sheldrick, G. M. (1996). SADABS. University of Göttingen, Germany.
Figure 2. Analysis of Mg deposition on Al foil using 0.3 M Mg(OTf)2 + 0.2 M MgCl2 in DME electrolyte.
Figure 3. Galvanostatic cycling of Mg//Al at different current densities and areal capacities using 0.3 M Mg(OTf)2 + 0.2 M MgCl2 in DME.
(A) Voltage profile and (B) Coulombic efficiency of cell cycled with current densities from 0.5 - 3.0 mA cm-2 at 0.5 mAh cm-2.
Figure 4. Electrochemical characterization of Mg//Mg symmetric cell using 0.3 M Mg(OTf)2 + 0.2 M MgCl2 in DME.
(C-E) Expanded voltage profile of (A) at (C) 0-10 h, (D) 250-260 h, and (E) 490-500 h. (F) Nyquist plots of Mg//Mg symmetric cell at various points during cycling.
(G) Expanded Nyquist plots at high-frequency region.
Figure 5. Morphology of Mg electrodes from a Mg//Mg symmetric cell after cycling in 0.3 M Mg(OTf)2 + 0.2 M MgCl2 in DME after plating or stripping at 0.5 mA cm-2 for 6 h (3 mAh cm-2).
(A-B) SEM images of Mg electrode after plating. (C-D) SEM image of Mg electrode after stripping.
Figure 7. Cycling of Mg//Mo6S8 full cell using 0.3 M Mg(OTf)2 + 0.2 M MgCl2 in DME at 0.1 C and voltage window of 0.2 - 2.2 V.
(A) Voltage profile.
Figure 8. Refined SCXRD structure for Mg(DME)2(OTf)2 single crystal, recrystallized from 1.5 M Mg(OTf)2 + 1 M MgCl2 in DME solution.
Figure 9. Raman spectra of various Mg(OTf)2-containing solutions and reference samples. (A) DME solvent only
(B) 0.75 M Mg(TFSI)2 in DME (C) Mg(OTf)2 powder
(D) [BMIM][OTf]-DME mixture solution (1:5 vol. ratio) (E) Saturated solution of Mg(OTf)2 in DME